#------------------------------------------------------------------------------
#$Date: 2016-03-23 00:29:17 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179113 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/75/4307587.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4307587
loop_
_publ_author_name
'Samuel J. Mugavero'
'Mark D. Smith'
'Hans-Conrad zur Loye'
_publ_contact_author_address
;
Department of Chemistry and Biochemistry
University of South Carolina
Columbia, SC  29208
USA
;
_publ_contact_author_email       zurloye@sc.edu
_publ_contact_author_fax         '803 777 8508'
_publ_contact_author_name        'Professor Hans-Conrad zur Loye'
_publ_contact_author_phone       '803 777 6916'
_publ_section_title
;
Crystal Growth and Structural Characterization of the New Ordered
Palladates LnKPdO3 (Ln = La, Pr, Nd, Sm-Gd) and the Isostructural,
Partially Cu-Substituted Palladate PrK(Cu0.14Pd0.86)O3
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3116
_journal_page_last               3122
_journal_paper_doi               10.1021/ic062066m
_journal_volume                  46
_journal_year                    2007
_chemical_formula_moiety         'K O3 Pd Pr'
_chemical_formula_sum            'K O3 Pd Pr'
_chemical_formula_weight         334.41
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 105.1580(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.2620(5)
_cell_length_b                   3.9576(2)
_cell_length_c                   7.3865(3)
_cell_measurement_reflns_used    2666
_cell_measurement_temperature    294(2)
_cell_measurement_theta_max      32.465
_cell_measurement_theta_min      2.857
_cell_volume                     374.20(3)
_computing_cell_refinement       'SAINT+ NT V6.22 (Bruker, 2001)'
_computing_data_collection       'SMART NT V5.625 (Bruker, 1998)'
_computing_data_reduction        'SAINT+ NT V6.22'
_computing_molecular_graphics    'SHELXTL V6.1 (Sheldrick, 2000)'
_computing_publication_material  'SHELXTL V6.1'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      294(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0278
_diffrn_reflns_av_sigmaI/netI    0.0198
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            4041
_diffrn_reflns_theta_full        32.57
_diffrn_reflns_theta_max         32.57
_diffrn_reflns_theta_min         2.86
_diffrn_standards_decay_%        0
_exptl_absorpt_coefficient_mu    18.608
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.5177
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS, Bruker, 2001)'
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    5.936
_exptl_crystal_density_meas      5.94
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             592
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.02
_refine_diff_density_max         0.978
_refine_diff_density_min         -1.180
_refine_diff_density_rms         0.226
_refine_ls_extinction_coef       0.0060(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.086
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     38
_refine_ls_number_reflns         765
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.086
_refine_ls_R_factor_all          0.0165
_refine_ls_R_factor_gt           0.0156
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0191P)²+0.6210P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0377
_refine_ls_wR_factor_ref         0.0383
_reflns_number_gt                734
_reflns_number_total             765
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic062066msi20061029_033041.cif
_cod_data_source_block           PrKPdO3
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               4307587
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Pr1 Pr 0.650517(15) 0.0000 0.08103(3) 0.00844(8) Uani 1 2 d S . .
Pd1 Pd 0.006646(19) 0.0000 0.77746(4) 0.00734(8) Uani 1 2 d S . .
K1 K 0.35751(7) 0.0000 0.43559(12) 0.01450(17) Uani 1 2 d S . .
O1 O 0.8322(2) 0.0000 0.1330(4) 0.0111(5) Uani 1 2 d S . .
O2 O 0.4938(2) 0.0000 0.1989(4) 0.0129(5) Uani 1 2 d S . .
O3 O 0.1515(2) 0.0000 0.2801(4) 0.0099(5) Uani 1 2 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pr Pr -0.2180 2.8214 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pd Pd -0.9988 1.0072 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Pr1 O2 133.63(10) . 5_655 ?
O1 Pr1 O2 150.87(9) . . ?
O2 Pr1 O2 75.50(11) 5_655 . ?
O1 Pr1 O3 93.31(7) . 3 ?
O2 Pr1 O3 112.90(7) 5_655 3 ?
O2 Pr1 O3 70.19(7) . 3 ?
O1 Pr1 O3 93.31(7) . 3_545 ?
O2 Pr1 O3 112.90(7) 5_655 3_545 ?
O2 Pr1 O3 70.19(7) . 3_545 ?
O3 Pr1 O3 106.90(10) 3 3_545 ?
O1 Pr1 O1 81.24(7) . 7_645 ?
O2 Pr1 O1 69.75(7) 5_655 7_645 ?
O2 Pr1 O1 115.88(6) . 7_645 ?
O3 Pr1 O1 173.93(8) 3 7_645 ?
O3 Pr1 O1 76.24(7) 3_545 7_645 ?
O1 Pr1 O1 81.24(7) . 7_655 ?
O2 Pr1 O1 69.75(7) 5_655 7_655 ?
O2 Pr1 O1 115.88(6) . 7_655 ?
O3 Pr1 O1 76.24(7) 3 7_655 ?
O3 Pr1 O1 173.93(8) 3_545 7_655 ?
O1 Pr1 O1 100.17(9) 7_645 7_655 ?
O1 Pr1 Pd1 120.81(5) . 3_544 ?
O2 Pr1 Pd1 38.073(6) 5_655 3_544 ?
O2 Pr1 Pd1 81.04(5) . 3_544 ?
O3 Pr1 Pd1 145.07(6) 3 3_544 ?
O3 Pr1 Pd1 80.30(5) 3_545 3_544 ?
O1 Pr1 Pd1 39.88(6) 7_645 3_544 ?
O1 Pr1 Pd1 100.15(5) 7_655 3_544 ?
O1 Pr1 Pd1 120.81(5) . 3_554 ?
O2 Pr1 Pd1 38.073(6) 5_655 3_554 ?
O2 Pr1 Pd1 81.04(5) . 3_554 ?
O3 Pr1 Pd1 80.30(5) 3 3_554 ?
O3 Pr1 Pd1 145.07(6) 3_545 3_554 ?
O1 Pr1 Pd1 100.15(5) 7_645 3_554 ?
O1 Pr1 Pd1 39.88(6) 7_655 3_554 ?
Pd1 Pr1 Pd1 75.929(8) 3_544 3_554 ?
O1 Pr1 Pd1 132.02(4) . 7_546 ?
O2 Pr1 Pd1 81.03(5) 5_655 7_546 ?
O2 Pr1 Pd1 37.767(6) . 7_546 ?
O3 Pr1 Pd1 101.63(5) 3 7_546 ?
O3 Pr1 Pd1 38.74(6) 3_545 7_546 ?
O1 Pr1 Pd1 84.08(5) 7_645 7_546 ?
O1 Pr1 Pd1 146.51(6) 7_655 7_546 ?
Pd1 Pr1 Pd1 62.270(9) 3_544 7_546 ?
Pd1 Pr1 Pd1 106.638(7) 3_554 7_546 ?
O1 Pr1 Pd1 132.02(4) . 7_556 ?
O2 Pr1 Pd1 81.03(5) 5_655 7_556 ?
O2 Pr1 Pd1 37.767(6) . 7_556 ?
O3 Pr1 Pd1 38.74(6) 3 7_556 ?
O3 Pr1 Pd1 101.63(5) 3_545 7_556 ?
O1 Pr1 Pd1 146.51(6) 7_645 7_556 ?
O1 Pr1 Pd1 84.08(5) 7_655 7_556 ?
Pd1 Pr1 Pd1 106.638(7) 3_544 7_556 ?
Pd1 Pr1 Pd1 62.270(9) 3_554 7_556 ?
Pd1 Pr1 Pd1 75.311(8) 7_546 7_556 ?
O1 Pr1 K1 97.68(7) . 5_656 ?
O2 Pr1 K1 128.68(7) 5_655 5_656 ?
O2 Pr1 K1 53.18(7) . 5_656 ?
O3 Pr1 K1 53.48(5) 3 5_656 ?
O3 Pr1 K1 53.48(5) 3_545 5_656 ?
O1 Pr1 K1 129.65(5) 7_645 5_656 ?
O1 Pr1 K1 129.65(5) 7_655 5_656 ?
Pd1 Pr1 K1 121.698(11) 3_544 5_656 ?
Pd1 Pr1 K1 121.698(11) 3_554 5_656 ?
Pd1 Pr1 K1 59.437(11) 7_546 5_656 ?
Pd1 Pr1 K1 59.437(11) 7_556 5_656 ?
O2 Pd1 O2 169.83(17) 7_556 7_546 ?
O2 Pd1 O3 89.54(8) 7_556 5_556 ?
O2 Pd1 O3 89.54(8) 7_546 5_556 ?
O2 Pd1 O1 89.90(8) 7_556 5_656 ?
O2 Pd1 O1 89.90(8) 7_546 5_656 ?
O3 Pd1 O1 173.66(12) 5_556 5_656 ?
O2 Pd1 Pr1 48.76(8) 7_556 3_456 ?
O2 Pd1 Pr1 124.49(8) 7_546 3_456 ?
O3 Pd1 Pr1 122.58(5) 5_556 3_456 ?
O1 Pd1 Pr1 53.22(5) 5_656 3_456 ?
O2 Pd1 Pr1 124.49(8) 7_556 3_446 ?
O2 Pd1 Pr1 48.76(8) 7_546 3_446 ?
O3 Pd1 Pr1 122.58(5) 5_556 3_446 ?
O1 Pd1 Pr1 53.22(5) 5_656 3_446 ?
Pr1 Pd1 Pr1 75.929(8) 3_456 3_446 ?
O2 Pd1 Pr1 124.29(8) 7_556 7_546 ?
O2 Pd1 Pr1 49.18(8) 7_546 7_546 ?
O3 Pd1 Pr1 49.47(5) 5_556 7_546 ?
O1 Pd1 Pr1 126.58(5) 5_656 7_546 ?
Pr1 Pd1 Pr1 117.731(9) 3_456 7_546 ?
Pr1 Pd1 Pr1 73.363(7) 3_446 7_546 ?
O2 Pd1 Pr1 49.18(8) 7_556 7_556 ?
O2 Pd1 Pr1 124.29(8) 7_546 7_556 ?
O3 Pd1 Pr1 49.47(5) 5_556 7_556 ?
O1 Pd1 Pr1 126.58(5) 5_656 7_556 ?
Pr1 Pd1 Pr1 73.363(7) 3_456 7_556 ?
Pr1 Pd1 Pr1 117.731(9) 3_446 7_556 ?
Pr1 Pd1 Pr1 75.310(8) 7_546 7_556 ?
O2 Pd1 K1 57.63(8) 7_556 7_556 ?
O2 Pd1 K1 130.30(8) 7_546 7_556 ?
O3 Pd1 K1 123.91(6) 5_556 7_556 ?
O1 Pd1 K1 60.64(6) 5_656 7_556 ?
Pr1 Pd1 K1 70.656(15) 3_456 7_556 ?
Pr1 Pd1 K1 113.505(17) 3_446 7_556 ?
Pr1 Pd1 K1 170.899(19) 7_546 7_556 ?
Pr1 Pd1 K1 105.213(10) 7_556 7_556 ?
O2 Pd1 K1 130.30(8) 7_556 7_546 ?
O2 Pd1 K1 57.63(8) 7_546 7_546 ?
O3 Pd1 K1 123.91(6) 5_556 7_546 ?
O1 Pd1 K1 60.64(6) 5_656 7_546 ?
Pr1 Pd1 K1 113.505(17) 3_456 7_546 ?
Pr1 Pd1 K1 70.656(15) 3_446 7_546 ?
Pr1 Pd1 K1 105.213(10) 7_546 7_546 ?
Pr1 Pd1 K1 170.899(19) 7_556 7_546 ?
K1 Pd1 K1 72.796(18) 7_556 7_546 ?
O2 Pd1 K1 129.02(8) 7_556 3_445 ?
O2 Pd1 K1 58.12(8) 7_546 3_445 ?
O3 Pd1 K1 58.42(6) 5_556 3_445 ?
O1 Pd1 K1 126.11(6) 5_656 3_445 ?
Pr1 Pd1 K1 176.572(13) 3_456 3_445 ?
Pr1 Pd1 K1 106.448(9) 3_446 3_445 ?
Pr1 Pd1 K1 65.560(14) 7_546 3_445 ?
Pr1 Pd1 K1 107.240(15) 7_556 3_445 ?
K1 Pd1 K1 105.998(14) 7_556 3_445 ?
K1 Pd1 K1 65.53(2) 7_546 3_445 ?
O2 Pd1 K1 58.12(8) 7_556 3_455 ?
O2 Pd1 K1 129.02(8) 7_546 3_455 ?
O3 Pd1 K1 58.42(6) 5_556 3_455 ?
O1 Pd1 K1 126.11(6) 5_656 3_455 ?
Pr1 Pd1 K1 106.448(9) 3_456 3_455 ?
Pr1 Pd1 K1 176.572(13) 3_446 3_455 ?
Pr1 Pd1 K1 107.240(15) 7_546 3_455 ?
Pr1 Pd1 K1 65.560(14) 7_556 3_455 ?
K1 Pd1 K1 65.53(2) 7_556 3_455 ?
K1 Pd1 K1 105.998(14) 7_546 3_455 ?
K1 Pd1 K1 71.069(17) 3_445 3_455 ?
O3 K1 O2 118.79(9) . . ?
O3 K1 O2 140.43(9) . 5_656 ?
O2 K1 O2 100.78(8) . 5_656 ?
O3 K1 O3 94.59(7) . 7_556 ?
O2 K1 O3 126.90(6) . 7_556 ?
O2 K1 O3 58.26(6) 5_656 7_556 ?
O3 K1 O3 94.59(7) . 7_546 ?
O2 K1 O3 126.90(6) . 7_546 ?
O2 K1 O3 58.26(6) 5_656 7_546 ?
O3 K1 O3 85.66(8) 7_556 7_546 ?
O3 K1 O1 76.84(7) . 3_445 ?
O2 K1 O1 59.56(6) . 3_445 ?
O2 K1 O1 128.57(5) 5_656 3_445 ?
O3 K1 O1 171.40(8) 7_556 3_445 ?
O3 K1 O1 94.19(6) 7_546 3_445 ?
O3 K1 O1 76.84(7) . 3_455 ?
O2 K1 O1 59.56(6) . 3_455 ?
O2 K1 O1 128.57(6) 5_656 3_455 ?
O3 K1 O1 94.19(6) 7_556 3_455 ?
O3 K1 O1 171.40(8) 7_546 3_455 ?
O1 K1 O1 84.67(8) 3_445 3_455 ?
O3 K1 Pd1 114.51(5) . 7_556 ?
O2 K1 Pd1 36.457(9) . 7_556 ?
O2 K1 Pd1 96.87(5) 5_656 7_556 ?
O3 K1 Pd1 93.80(4) 7_556 7_556 ?
O3 K1 Pd1 150.82(6) 7_546 7_556 ?
O1 K1 Pd1 90.51(5) 3_445 7_556 ?
O1 K1 Pd1 37.78(5) 3_455 7_556 ?
O3 K1 Pd1 114.51(5) . 7_546 ?
O2 K1 Pd1 36.457(9) . 7_546 ?
O2 K1 Pd1 96.87(5) 5_656 7_546 ?
O3 K1 Pd1 150.82(6) 7_556 7_546 ?
O3 K1 Pd1 93.80(4) 7_546 7_546 ?
O1 K1 Pd1 37.78(5) 3_445 7_546 ?
O1 K1 Pd1 90.51(5) 3_455 7_546 ?
Pd1 K1 Pd1 72.795(18) 7_556 7_546 ?
O3 K1 Pd1 130.47(4) . 3 ?
O2 K1 Pd1 96.75(5) . 3 ?
O2 K1 Pd1 35.609(9) 5_656 3 ?
O3 K1 Pd1 36.41(5) 7_556 3 ?
O3 K1 Pd1 89.16(5) 7_546 3 ?
O1 K1 Pd1 152.17(6) 3_445 3 ?
O1 K1 Pd1 95.82(4) 3_455 3 ?
Pd1 K1 Pd1 74.001(15) 7_556 3 ?
Pd1 K1 Pd1 114.46(2) 7_546 3 ?
O3 K1 Pd1 130.47(4) . 3_545 ?
O2 K1 Pd1 96.75(5) . 3_545 ?
O2 K1 Pd1 35.609(10) 5_656 3_545 ?
O3 K1 Pd1 89.16(5) 7_556 3_545 ?
O3 K1 Pd1 36.41(5) 7_546 3_545 ?
O1 K1 Pd1 95.82(4) 3_445 3_545 ?
O1 K1 Pd1 152.17(6) 3_455 3_545 ?
Pd1 K1 Pd1 114.46(2) 7_556 3_545 ?
Pd1 K1 Pd1 74.001(14) 7_546 3_545 ?
Pd1 K1 Pd1 71.069(18) 3 3_545 ?
O3 K1 Pr1 97.72(6) . 5_656 ?
O2 K1 Pr1 143.49(6) . 5_656 ?
O2 K1 Pr1 42.71(6) 5_656 5_656 ?
O3 K1 Pr1 42.85(4) 7_556 5_656 ?
O3 K1 Pr1 42.85(4) 7_546 5_656 ?
O1 K1 Pr1 136.68(4) 3_445 5_656 ?
O1 K1 Pr1 136.68(4) 3_455 5_656 ?
Pd1 K1 Pr1 128.89(2) 7_556 5_656 ?
Pd1 K1 Pr1 128.89(2) 7_546 5_656 ?
Pd1 K1 Pr1 55.004(13) 3 5_656 ?
Pd1 K1 Pr1 55.004(13) 3_545 5_656 ?
Pd1 O1 Pr1 171.10(14) 5_656 . ?
Pd1 O1 Pr1 86.90(8) 5_656 7_645 ?
Pr1 O1 Pr1 98.76(7) . 7_645 ?
Pd1 O1 Pr1 86.90(8) 5_656 7_655 ?
Pr1 O1 Pr1 98.76(7) . 7_655 ?
Pr1 O1 Pr1 100.17(9) 7_645 7_655 ?
Pd1 O1 K1 81.58(7) 5_656 3 ?
Pr1 O1 K1 91.87(8) . 3 ?
Pr1 O1 K1 166.39(10) 7_645 3 ?
Pr1 O1 K1 86.491(19) 7_655 3 ?
Pd1 O1 K1 81.58(7) 5_656 3_545 ?
Pr1 O1 K1 91.87(8) . 3_545 ?
Pr1 O1 K1 86.491(19) 7_645 3_545 ?
Pr1 O1 K1 166.39(10) 7_655 3_545 ?
K1 O1 K1 84.68(8) 3 3_545 ?
Pd1 O2 Pd1 169.83(17) 7_556 7_546 ?
Pd1 O2 Pr1 93.17(8) 7_556 5_655 ?
Pd1 O2 Pr1 93.17(8) 7_546 5_655 ?
Pd1 O2 Pr1 93.05(8) 7_556 . ?
Pd1 O2 Pr1 93.05(8) 7_546 . ?
Pr1 O2 Pr1 104.50(11) 5_655 . ?
Pd1 O2 K1 85.91(8) 7_556 . ?
Pd1 O2 K1 85.91(8) 7_546 . ?
Pr1 O2 K1 92.17(9) 5_655 . ?
Pr1 O2 K1 163.33(12) . . ?
Pd1 O2 K1 86.27(8) 7_556 5_656 ?
Pd1 O2 K1 86.27(8) 7_546 5_656 ?
Pr1 O2 K1 171.40(12) 5_655 5_656 ?
Pr1 O2 K1 84.10(8) . 5_656 ?
K1 O2 K1 79.22(8) . 5_656 ?
Pd1 O3 Pr1 91.79(8) 5_556 3_445 ?
Pd1 O3 Pr1 91.79(8) 5_556 3_455 ?
Pr1 O3 Pr1 106.90(10) 3_445 3_455 ?
Pd1 O3 K1 167.15(14) 5_556 . ?
Pr1 O3 K1 95.84(7) 3_445 . ?
Pr1 O3 K1 95.84(7) 3_455 . ?
Pd1 O3 K1 85.17(7) 5_556 7_556 ?
Pr1 O3 K1 169.12(9) 3_445 7_556 ?
Pr1 O3 K1 83.669(19) 3_455 7_556 ?
K1 O3 K1 85.41(7) . 7_556 ?
Pd1 O3 K1 85.17(7) 5_556 7_546 ?
Pr1 O3 K1 83.669(19) 3_445 7_546 ?
Pr1 O3 K1 169.12(9) 3_455 7_546 ?
K1 O3 K1 85.41(7) . 7_546 ?
K1 O3 K1 85.66(8) 7_556 7_546 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Pr1 O1 2.339(3) . ?
Pr1 O2 2.422(3) 5_655 ?
Pr1 O2 2.455(3) . ?
Pr1 O3 2.4631(16) 3 ?
Pr1 O3 2.4631(16) 3_545 ?
Pr1 O1 2.5800(18) 7_645 ?
Pr1 O1 2.5800(18) 7_655 ?
Pr1 Pd1 3.2167(3) 3_544 ?
Pr1 Pd1 3.2166(3) 3_554 ?
Pr1 Pd1 3.2391(3) 7_546 ?
Pr1 Pd1 3.2391(3) 7_556 ?
Pr1 K1 3.5998(9) 5_656 ?
Pd1 O2 1.9866(3) 7_556 ?
Pd1 O2 1.9866(3) 7_546 ?
Pd1 O3 2.028(3) 5_556 ?
Pd1 O1 2.065(3) 5_656 ?
Pd1 Pr1 3.2167(3) 3_456 ?
Pd1 Pr1 3.2167(3) 3_446 ?
Pd1 Pr1 3.2391(3) 7_546 ?
Pd1 Pr1 3.2391(3) 7_556 ?
Pd1 K1 3.3347(7) 7_556 ?
Pd1 K1 3.3347(7) 7_546 ?
Pd1 K1 3.4047(7) 3_445 ?
Pd1 K1 3.4047(7) 3_455 ?
K1 O3 2.673(3) . ?
K1 O2 2.824(3) . ?
K1 O2 2.897(3) 5_656 ?
K1 O3 2.911(2) 7_556 ?
K1 O3 2.911(2) 7_546 ?
K1 O1 2.938(2) 3_445 ?
K1 O1 2.938(2) 3_455 ?
K1 Pd1 3.3348(7) 7_556 ?
K1 Pd1 3.3348(7) 7_546 ?
K1 Pd1 3.4047(7) 3 ?
K1 Pd1 3.4047(7) 3_545 ?
K1 Pr1 3.5998(9) 5_656 ?
O1 Pd1 2.065(3) 5_656 ?
O1 Pr1 2.5800(18) 7_645 ?
O1 Pr1 2.5800(18) 7_655 ?
O1 K1 2.938(2) 3 ?
O1 K1 2.938(2) 3_545 ?
O2 Pd1 1.9866(3) 7_556 ?
O2 Pd1 1.9866(3) 7_546 ?
O2 Pr1 2.422(3) 5_655 ?
O2 K1 2.897(3) 5_656 ?
O3 Pd1 2.028(3) 5_556 ?
O3 Pr1 2.4632(16) 3_445 ?
O3 Pr1 2.4632(16) 3_455 ?
O3 K1 2.911(2) 7_556 ?
O3 K1 2.911(2) 7_546 ?
